| ||Format||Pages||Price|| |
|PDF Version||3||$37.00||  ADD TO CART|
|Print Version||3||$37.00||  ADD TO CART|
Significance and Use
This test method provides a means for determining the modulus of rupture of a square cross section graphite specimen machined from the electrode core sample obtained according to Practice C783, with a minimum core diameter of 57 mm. This test method is recommended for quality control or quality assurance purposes, but should not be relied upon to compare materials of radically different particle sizes or orientational characteristics. For these reasons as well as those discussed in 4.2 an absolute value of flexural strength may not be obtained.
Specimen Size—The maximum particle size and maximum pore size vary greatly for manufactured graphite electrodes, generally increasing with electrode diameter. The test is on a rather short stubby beam, therefore the shear stress is not insignificant compared to the flexural stress, and the test results may not agree when a different ratio or specimen size is used.
1.1 This test method covers determination of the modulus of rupture in bending of specimens cut from graphite electrodes using a simple square cross section beam in four-point loading at room temperature.
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C651 Test Method for Flexural Strength of Manufactured Carbon and Graphite Articles Using Four-Point Loading at Room Temperature
C709 Terminology Relating to Manufactured Carbon and Graphite
C783 Practice for Core Sampling of Graphite Electrodes
E4 Practices for Force Verification of Testing Machines
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
ICS Number Code 71.100.99 (Other products of the chemical industry)